Structural and magnetic properties of
J. Voigt1,2,a, E. Kentzinger1, U. R¨ucker1, W. Schweika1, D. Wermeille3, W. Schmidt1,4, and Th. Br¨uckel1 1 Institut f¨ur Festk¨orperforschung, Forschungszentrum J¨ulich GmbH, 52425 J¨ulich, Germany
2 Labor f¨ur Neutronenstreuung, Paul Scherrer Institut, 5232 Villigen-PSI, Switzerland
3 Ames Laboratory-US DOE and Department of Physics and Astronomy, Iowa State University, Ames, Iowa 50011, USA 4 Institute Laue-Langevin, B.P. 156, 38042 Grenoble Cedex 9, France
Received 20 September 2004 / Received in ﬁnal form 17 October 2005
Published online 31 March 2006 – c EDP Sciences, Societ`a Italiana di Fisica, Springer-Verlag 2006 Abstract. We have investigated the structural and magnetic properties of [Er|Tb] multilayers by diﬀerent scattering methods. Diﬀuse X-ray scattering under grazing incidence reveals the interface structure in [Er|Tb] bilayers and trilayers, indicating vertically correlated roughness between the Er and Tb interfaces. The magnetic properties of [ErnEr|TbnTb] superlattices have been studied as a function of the superlattice composition (indices denote the number of atomic layers). Coupled ferromagnetic structures exist in all investigated samples. The phase transition temperature varies with the Tb layer thickness. Modulated magnetic order is short range for all samples beside the [Er20|Tb5] superlattice, the sample with the smallest Tb layer thickness. We observe dipolar antiferromagnetic coupling between single ferromagnetic Tb layers in all samples, with the onset of this ordering depending on the Tb layer thickness. Due to competing interactions, exchange coupling is limited to the interface near region. Therefore long range modulated magnetic order is observed in the [Er20|Tb5] superlattice only, where the interface regions overlap. The distinct diﬀerences to the magnetic structure of an Er0.8Tb0.2 alloy ﬁlm are explained by a highly anisotropic arrangement of neighbouring atoms due to the correlated roughness.
PACS. 75.75.+a Magnetic properties of nanostructures – 75.25.+z Spin arrangements in magnetically ordered materials (including neutron and spin-polarized electron studies, synchrotron-source
X-ray scattering, etc.) – 61.18.Fs Magnetic resonance techniques; Mossbauer spectroscopy
The discovery of magnetic interlayer exchange cou-pling [1, 2] initiated strong research activities in the ﬁeld of rare earth superlattices. A comprehensive review of the diﬀerent coupling mechanisms is given in . Most stud-ies are concerned with the exchange coupling across non magnetic spacers. More recent studies report on systems containing two magnetic rare earth metals [4–7] showing a variety of new magnetic phases.
The present study concerns the system [Er|Tb]. Mainly as a result of the crystal ﬁeld anisotropy, the two elements Er and Tb exhibit fairly diﬀerent magnetic structures in the bulk. Therefore one might expect complex magnetic structures in superlattices composed from these materials. We attempt to clarify the role of competing anisotropies and proximity by a systematic variation of the superlattice composition.
The magnetic structure in rare earth elements is determined by the subtle balance between RKKY inter-action, crystal ﬁeld anisotropy and magneto-elastic in-teractions. The RKKY interaction, i.e. the coupling of
a e-mail: firstname.lastname@example.org
localised 4f magnetic moments via conduction band elec-trons, leads to the formation of modulated magnetic struc-tures throughout the series of heavy rare earth metals.
For Tb metal, the crystal ﬁeld anisotropy forces the magnetic moments to lie within the basal plane of the hexagonal lattice. In contrast, the magnetic moments are oriented preferably along the c-axis direction in Er. Phase transition temperatures diﬀer strongly for the two ele-ments. The N´eel temperature TN for Tb is about 230 K. The basal plane helix is stable only in the small tempera-ture range above 220 K. Below 220 K Tb is a simple basal plane ferromagnet.
Upon cooling, bulk Er orders ﬁrst at TN = 81 K in a so called c-axis modulated structure, i.e. the mag-netic moments are aligned along the c-direction, the size of the moment is identical in a given hexagonal basal plane and modulated sinusoidally along the c-direction. Below 54 K the basal plane component orders into a mod-ulated structure with the same propagation vector. The magnetic modulation is not any more purely sinusoidal, but ‘squares up’ instead . Between 34 K and 20 K the propagation vector locks in into a series of commensurate values. Finally, below 20 K, the c-axis component becomes
Table 1. Structural parameters of the diﬀerent superlattices deduced from XRD. The values are results from modelling with the ‘Suprex’ program, see reference  for details. D is the bilayer thickness, cEr and cTb are the c-axis lattice parameters within the Er and Tb layers, respectively. Additionally the mosaic spread is given.
Sample # of bilayers nEr nTb D [˚A] cEr [˚A] cTb[˚A] Mosaic spread FWHM [◦] [Er22|Tb22] 80 22.2(3) 22.0(3) 124.5(5) 5.556(1) 5.714(2) 0.20
[Er20|Tb10] 63 19.6(1) 10.8(1) 85.0(5) 5.574(1) 5.708(2) 0.24 [Er20|Tb5] 150 21.2(3) 5.0(3) 73.5(5) 5.590(1) 5.72(1) 0.21
[Er5|Tb20] 120 73(2) 0.20
ferromagnetic, while the basal plane component remains in a modulated order, yielding a cone structure.
The present paper is organised as follows: in Section 2 we describe the sample preparation. The structural char-acterisation in Section 3 was performed by means of X-ray scattering. Anomalous specular and oﬀ-specular X-ray scattering under grazing incidence reveals the interface morphologies, while wide angle X-ray diﬀraction is used to probe the crystal quality. In Section 4 we describe the magnetic structures determined by neutron diﬀraction. The X-ray resonance exchange scattering (XRES) data in Section 5 provides element and electronic band speciﬁc in-formation about the magnetic properties. Combining the results of neutron diﬀraction and XRES we propose dif-ferent coupling mechanisms for the series of superlattices in Section 6.
2 Sample preparation
Samples were prepared by means of molecular beam epitaxy (MBE). Following the approach described by Majkrzak et al. , the rare earth metal layers are deposited onto a buﬀer system [Sapphire(1120)
|Nb(110)|Y(0001)] with ﬂat and clean Y (0001) surfaces.
The layer thicknesses range from 250 to 1500 ˚A for the Nb layers and 600 to 1200 ˚A for the Y layer. The surface qual-ity is controlled in situ by Low Energy Electron Diﬀraction (LEED) and Auger Electron Spectroscopy (AES). From AES, strong interdiﬀusion is found at Tb|Er interfaces at growth temperatures above 350◦C. For growth tempera-tures below 270◦C epitaxial growth of Er is suppressed as evidenced from the missing LEED pattern. Growth tem-peratures between 300 and 350◦C yield very good epitaxy, while interdiﬀusion cannot be the detected by AES. How-ever, the sensitivity of AES is limited: taking into account the chemical sensitivity this limits the surface coverage to 10% for the ‘buried’ element.
To protect the rare earth layers from oxidation a ﬁnal cap layer is deposited. For the grazing incidence measure-ments we use a 50 ˚A thick SiO layer (cp. ), while the superlattices for the magnetic studies are capped with a 200–300 ˚A thick Y layer .
For the interface characterisation we use bilayers and trilayers to keep the number of interfaces low. The struc-tural properties of the superlattices used for the magnetic studies are summarised in Table 1. For comparison with
0 0.1 0.2 0.3 0.4 0.5 Qz [Å-1] 10-2 100 102 104
Norm. Int. [arb. un.]
αi=2θ/2 data αi=2θ/2-∆ data αi=2θ/2 fit αi=2θ/2-∆ fit E=7 keV a) Er|Tb 0 0.1 0.2 0.3 0.4 0.5 Qz [Å-1] 10-2 100 102 104
Norm. Int. [arb. un.]
αi=2θ/2 data αi=2θ/2-∆ data αi=2θ/2 fit αi=2θ/2-∆ fit E=7.511 keV b) Er
Fig. 1. Reﬂectivity (αi = 2θ2) and longitudinal diﬀuse scat-tering (αi=2θ2 − ∆) from an [Er43.5˚A|Tb36.1˚A] bilayer capped with SiO measured at E = 7 keV (a) and E = 7.511 keV (b) as a function of Qz. For small angles ∆, Qz is given as:
Qz ≈ 2k sin2θ2. ∆Qz corresponding to the thickness of the Er layer and the [Er|Tb] bilayer is indicated.
the diﬀerent superlattices we produced a 6000 ˚A thick Er0.8Tb0.2 alloy by coevaporation of Er and Tb directly onto the Nb buﬀer layer.
3 Structural characterisation
The interface properties of [Er|Tb]-bilayers and [Tb|Er|Tb]-trilayers have been investigated by dif-fuse X-ray scattering under grazing incidence. Figure 1 shows measurements of the reﬂectivity (i.e. αi= αf = 2θ2) and longitudinal diﬀuse scans (i.e. αi = 2θ2 − ∆) for dif-ferent photon energies as a function of the Qz component
of the scattering vector, i.e. the component normal to the surface. αi, αf denote the angles between the sample surface and the incoming and outgoing X-ray beam, respectively. 2θ is the angle between incoming and outgoing beam and the oﬀset ∆ is typically 0.05◦.
In order to perform contrast variation measurements, the data were taken at the CEMO beamline of the HASYLAB, Hamburg. Measurements with the energy
E = 7.511 keV close to the Tb LIII absorption edge are
sensitive to the interfaces between Er and Tb layers, since the contrast between the elements is enhanced due to anomalous scattering. Measurements at E = 7 keV high-light the interface between Tb and the Y buﬀer layer, while the contrast between Er and Tb is low.
Using this contrast variation, the properties of the dif-ferent interfaces can be deduced. The results of the analy-sis of the reﬂectivity according to a Parratt formalism  conﬁrm the nominal composition of the multilayers and yield an interface width between the rare earth layers of 8 to 13 ˚A or 3 to 4.5 atomic layers in agreement with values reported for other rare earth superlattice systems [5, 13]. Similar values have been found for the superlattices by wide angle diﬀraction.
Beyond the reﬂectivity, the diﬀuse scattering at graz-ing incidence provides information on the lateral interface structure. Performing longitudinal diﬀuse scans, the scat-tering vector contains a component parallel to the sample surface. Therefore it probes lateral deviations from the ideal interface and their correlation within the interface or between diﬀerent interfaces .
The diﬀuse scattering is surprisingly weak given the large rms interface width as deduced from reﬂectivity. Since interdiﬀusion and roughness lead to the same later-ally averaged scattering length density proﬁle — as is mea-sured by reﬂectivity — while only the latter contributes to modulated diﬀuse scattering, we conclude that the inter-face width is partly due to interdiﬀusion. The discrepancy to the AES results can be understood, if the sensitivity of AES is taken into account. However, longitudinal cor-relations exist on diﬀerent length scales as seen from the diﬀerent oscillation in the longitudinal diﬀuse scans (see Fig. 1) from an [Er|Tb] bilayer. The energy independent short period oscillations are due to the Nb buﬀer layer. At lower Qz we observe two diﬀerent length scales: if the contrast between Er and Tb is large, it roughly equals the thickness of a single Er layer. If the contrast vanishes, it matches the total thickness of the Er|Tb bilayer. This shows, that the interfaces in the rare earth system exhibit correlated ﬂuctuations. Therefore, even the samples with layer thicknesses of 5 atomic layers have well separated Er and Tb layers.
We modeled the diﬀuse scattering data within the framework of the distorted wave Born approximation (DWBA) introduced by Sinha et al.  to the problem of surface roughness. This model was successfully applied to magnetic transition metal multilayers  and treats the interface broadening as roughness. Our reﬁnements for the [Er|Tb] system are less satisfactory, probably due to the neglect of interdiﬀusion.
60 65 70 2θ [°] 100 101 102 103 104 105 106
Norm. Int. [arb. units]
Data Refinement Y (0004)1 + (0004) (0004)2 + (0004)4 + (0004)6 + (0004)1 -(0004)2 -(0004)3 -(0004)4 -(0004)5 -(0004)6
-Fig. 2. XRD-scan and reﬁnement for the [Er22|Tb22] on a
logarithmic scale: the superlattice peaks can be reproduced up to the 6th order. The deviations between ﬁt and data close to the centre reﬂection might be due to thermal diﬀuse scattering, which is neglected in the model.
The [ErnEr|TbnTb] superlattices — nEr, nTbdenote the
layer thicknesses in mono-atomic layers — have been char-acterised by wide angle X-ray diﬀraction XRD. Perform-ing θ − 2θ scans on a Bruker AX 8 X-ray reﬂectometer at large angles provides information about the crystalline order along the surface normal at room temperature. Us-ing the approach of Schuller et al. [17–19], we deduce the respective cX lattice constants and averaged layer thick-nesses in the framework of the program ‘Suprex’ by E.E. Fullerton. An example of such a XRD-scan together with the reﬁnement is plotted for the [Er22|Tb22] superlattice in Figure 2. The results of this analysis are summarised in Table 1.
4 Magnetic structure
The magnetic phase diagram of the [ErnEr|TbnTb] super-lattices and the Er0.8Tb0.2 ﬁlm have been investigated by neutron diﬀraction.
Neutron diﬀraction experiments were performed at the IN12 instrument of the Institute Laue-Langevin in Greno-ble. The triple axis spectrometer provides a very low back-ground level, and is therefore perfectly suited for the ob-servation of small intensities as expected for scattering from thin ﬁlms. At a neutron wave vector of 1.5 ˚A−1, a cooled Be ﬁlter was used to suppress the λ/2 contamina-tion. The chosen collimator setup results in an instrumen-tal resolution of 0.0012 ˚A−1 (FWHM).
The neutron diﬀraction data from the Er0.8Tb0.2 alloy ﬁlm was collected at the DNS instrument of the research reactor FRJ2 in J¨ulich, which also provides a very good signal to noise ratio. At IN12 the samples were mounted into a LHe cryostat in order to vary the temperature be-tween 5 K and room temperature. The temperature was controlled during the measurements to an accuracy better than 1 K. In J¨ulich we employed a closed cycle cryostat spanning the temperature range from 10 to 300 K with a comparable accuracy.
0 2 220 K 0 2 75 K 1.7 1.8 1.9 2 2.1 Qz [r.l.u.] 0 2
norm. int. [arb. units]
22 K Y D* D* 1- 1+ -τ∗ -τ∗1+ -τ∗2+ -τ∗ 1-0.5- 0.5+ 1.5 -2.5 -τ∗
2-Fig. 3. Neutron diﬀraction from the [Er20|Tb5] sample as a function of the Qz component of the scattering vector: the sample exhibits long range modulated magnetic order (τ∗±l) and antiferromagnetic coupling (AFc) of ferromagnetic (FM) layers (2l2+1±). The (0002) Bragg reﬂection is cut for the sake of clarity.
The periodic alignment of the 4f magnetic moments leads to neutron scattering patterns as shown in Fig-ures 3, 5, if the scattering vector is scanned along [000Qz]. The central (0002) Bragg reﬂection is cut for clarity in Fig-ure 3. The observed reﬂections can be classiﬁed as follows:
– the epitaxial growth together with the superlattice
pe-riodicity leads to reﬂections (the z-direction is again normal to the surface) :
c is the averaged c-lattice parameter and D the
av-eraged bilayer thickness, l, l integers. For l = 0 the intensity depends on the contrast between Er and Tb layers, which is rather weak for nuclear scattering. The reﬂections are labelled with integers in Figures 3 and 5;
– the incommensurate magnetic modulations as known
from bulk rare earth elements produce reﬂections with a temperature dependent scattering vector:
Qz= 4πl c ± 2πl± Φ D = 4πl c ± τ∗±2πl D (2) Φ = bilayer i φi. (3)
φ represents the turn angle between neighbouring
monolayers, Φ the accumulated turn angle across one bilayer and τ∗ the respective propagation vec-tor modulo 2π. For the [Er20|Tb5] superlattice, these
reﬂections appear below 150 K. Using the model of Jehan  for temperatures 80 K < T < 150 K, the ob-served spectra can be reproduced assuming turn angles
φEr of 51 in the centre of a Er layer and φTb 18–23 in
the centre of a Tb layer (see Fig. 4). We had to ﬁx ei-ther of these parameters, since the correlation between
1.7 1.8 1.9 2 2.1 Qz [r.l.u.] 1×10-2 1×10-1 1×100 1×101
Norm. int. [arb.un.]
75 K data 75 K fit Y -τ∗ -τ∗1+ -τ∗2+ -τ∗ 1-τ∗
2-Fig. 4. Reﬁnement of the neutron diﬀraction along the [000l] direction at 75 K together with the data on a logarithmic scale, using the model of Jehan et al. .
0 0.5 100 K 0 0.5 70K 0 0.5
norm. int. [arb. un.]
40 K 1.7 1.75 1.8 1.85 Qz [r.l.u.] 0 0.5 10 K 2.5 -3.5 -4.5 -5.5 -6.5 -τ∗
Fig. 5. Neutron diﬀraction from the [Er22|Tb22] sample as a
function of the Qz component of the scattering vector: High order reﬂections due to AFc of FM layers (2l2+1±) and broad diﬀuse scattering due to short range modulated magnetic or-der (τ∗).
the two is very strong. A good agreement for all tem-peratures above 80 K could be found by ﬁxing the Er value to its bulk value at 80 K. The ﬁtted values of the Tb turn angle cover the same range as in the he-lix phase of bulk Tb. The very weak intensity of the
−τ∗1− satellite can be reproduced within this simple model only, if we assume a non vanishing magnetic mo-ment in both layers, Er and Tb. The magnetic momo-ment inside the Er layer is smaller than the moment in the Tb layer. Absolute values cannot be achieved, since the coherence length for nuclear and magnetic scattering diﬀer strongly. Therefore the magnetic intensity can-not be normalized to the nuclear one. To determine the averaged magnetization density within the layers, the intensity around a larger number of main Bragg reﬂections has to be measured.
If the modulation is not coupled across several bilay-ers, we observe instead broad diﬀuse intensity from
0 20 40 60 80 100 120 140 T [K] 0 0.1 0.2 0.3 0.4 I(1 0 1 -τ *)/I(0 0 0 2-τ *) a) 0 10 20 30 40 50 60 70 T [K] 0 0,5 1 1,5 2 2,5 3 3,5 4 mz [ µB ] mag. moment 0 10 20 30 40 50 60 70 T [K] 0 20 40 60 80
Int. Int. [arb. units.]
int. intensity b)
Fig. 6. (a) Ratio of the integrated intensities for the incommensurate magnetic reﬂections (101 − τ∗) and (0002− τ∗). The dashed line is a guide to the eye. (b) Integrated intensity of the (101) reﬂection and ferromagnitcally orderedc-axis component of the magnetic moment (right ordinate).
incoherent scattering of single layers (cf. Fig. 5). This intensity is centred around Qz deﬁned by
Qz= 4πl cX ± 2φ cX = 4πl cX ± τ ∗, (4)
cX denoting the c-lattice constant in the respective material and φ the phase angle between neighbour-ing atomic layers. Such a broad feature we observe in all superlattices containing Tb layers thicker than 5 atomic layers.
– Ferromagnetically ordered layers couple
antiferromag-netically. For this magnetic structure the superlattice periodicity is doubled:
2D . (5)
The respective reﬂections are labelled with half integer indices. These reﬂections appear in all superlattices. For the [Er20|Tb5] superlattice, they set in at tem-peratures below 60 K with a huge thermal hysteresis. They coexist with the τ∗l± peaks down to lowest tem-peratures, probably featuring ferromagnetic and heli-cal domains. For thicker Tb layers, the ferromagnetic order appears at T = 230 K, i.e. TN of bulk Tb. The diﬀerent components of the ordered magnetic moment can be separated by analysing the Q dependence of the magnetic reﬂections. Reﬂections of type (000Qz) contain only information about the basal plane magnetic moment, since only the component perpendicular to the scattering vector contributes to magnetic neutron scattering. Addi-tional measurements of (101Qz) reﬂections allows one to obtain the c-axis component. Long range ordering of the
c-axis component was found only for the Er0.8Tb0.2
al-loy and the [Er20|Tb5] superlattice. For the superlattice, we compared the intensities for the incommensurate peaks (101−τ∗) and (0002−τ∗), taking into account the Lorentz factor  and the magnetic form factor  (Fig. 6). Be-low 80 K the ratio increases due to the onset of the mod-ulated order of the c-axis component. At 20 K the ratio drops again, accompanied by a drastic increase of inten-sity of the (101) Bragg peak, featuring the transition to the
0 0.2 0.4 0.6 0.8 1 1.2 1.4
Norm. int. [arb. un.]
22 K (Norm. int.)/5 -0.4 -0.3 -0.2 -0.1 0 0.1 0.2 0.3 0.4 Q z [r.l.u.] 0 0.2 0.4 0.6 0.8 1 1.2 1.4
Norm. int. [arb. un.]
12 K (Norm. int.)/5 −τ∗ −τ∗1+ −τ∗2+ τ∗ τ∗1 -τ∗2 -τ∗1+ −τ∗1 -1- 1+
Fig. 7. Neutron diﬀraction spectra (101Qz) above and below the ferromagnetic ordering of thec-component of the magnetic moment. In the region−0.02 < Qz < 0.02 r.l.u., the intensity is divided by 5 for clarity.
cone structure. The width of this peak is purely deﬁned by the instrumental resolution like the nuclear Bragg peaks. By normalising to the nuclear scattering intensity we ﬁnd a ferromagnetically ordered c-axis moment of 3.5(3) µb, that is reduced from the bulk moment of 7.9 µB . We emphasise the long range order of the c-axis component, that leads to more intense superlattice satellites due to the increased contrast (see Fig. 7). In the case of the su-perlattice, the phase transition temperatures for the c-axis
cam Er FM FM cam+H ?H? FM H Tb [Er |Tb ]22 22 [Er |Tb ]5 20 + H + H 0000000000000000 00000000 00000000 11111111 11111111 11111111 11111111 000000000000000000 000000000000000000 000000000000000000 111111111111111111 111111111111111111 111111111111111111 Cone Temperature [K] 50 100 250 200 150 pm pm H cp. FM Cone sis tere− Hys− pm pm Hysteresis cp. cp. pm Cone Er Tb0.8 0.2 [Er |Tb ]20 5 pm cam cam cam H +
Fig. 8. Schematic phase diagram for the series of [Er|Tb] su-perlattices and the Er0.8Tb0.2alloy studied by wide angle neu-tron diﬀraction. CAM refers to thec-axis modulated structure and H to the pure helix. Long range coupled order is indicated by cp. For the [Er22|Tb22] sample, the combination of the CAM structure and the pure helix order is only short range.
component remain unchanged with respect to metallic Er and within the accuracy of the measurements (cp. Fig. 8). The sequence of the diﬀerent phases depends strongly on the composition of the superlattice. Magnetic phases and phase transition temperatures are summarized in the schematic phase diagram Figure 8 for our diﬀerent sam-ples and for the pure elements : the samsam-ples with a Tb thickness larger than 5 atomic layers order ferromag-netically within a single Tb layer, stacked in antiferro-magnetic order. The long range helix cannot be detected in these samples. The ferromagnetic transition tempera-ture is identical to the N´eel-temperature in bulk Tb. Long range modulated structures are found in the Er0.8Tb0.2
alloy and [Er20|Tb5] superlattice. A helical phase is ob-served below 150 K in the superlattice. At 80 K, i.e. TN of Er, an ordered c-axis component appears. This component orders ferromagnetically at TC= 20 K, approximately the
TCof bulk Er. The onset of a helical magnetic structure at a higher temperature than the onset of the c-axis modula-tion reminds on the phase diagram of ErxTb1−xalloys . Since the interfaces between Er and Tb are not atomically sharp and ﬂat, alloy like phases might be present at the interfaces. The magnetic properties of the [Er20|Tb5] su-perlattice are nevertheless substantially diﬀerent from the Er0.8Tb0.2 alloy, that contains the same relative amounts of Er and Tb.
X-ray resonance exchange scattering can occur, if the pho-ton energy is tuned close to some absorption edges of mag-netic elements . Complementary to neutron diﬀraction, XRES probes electronic states above the Fermi energy, which are spin polarised in magnetically ordered systems. It oﬀers a unique possibility to study the magnetic prop-erties of the superlattice element speciﬁc. XRES can be described as a second order perturbation process, which involves the virtual excitation of a core level electron into
3.6 3.8 4 4.2 4.4 Q z [r.l.u.] 10-5 10-4 10-3 10-2 10-1 100
Norm. int. [arb. units]
150 K 30 K Y 1+ τ* τ*1 + 1 -2 -3 -4 -2+ 5- 3+ 4+ τ*2 + 3.5+ Er LIII a) [Er20|Tb5] 1.8 1.9 2 2.1 2.2 Qz [r.l.u.] 10-5 10-4 10-3 10-2 10-1 100
Norm. int. [arb. units]
150 K 19 K -τ* 2.5 -Y & 0.5 -1.5 --τ*1 + 3 -2 -1 -2+ 1.5+ +τ*1 + 3+ +τ* 2.5+ 0.5+ Tb LIII 1 + b) [Er20|Tb5]
Fig. 9. XRES as a function of Qz measured in σ → π ge-ometry at diﬀerent temperatures, normalised to the maximum intensity: (a) XRES from the [Er20|Tb5] sample close to the Er LIII absorption edge (E = 8.361 keV); (b) XRES from the [Er20|Tb5] sample close to the Tb LIII absorption edge (E = 7.518 keV).
an empty state with subsequent decay and reemission of a photon . The scattered intensity depends on the den-sity of states above the Fermi level, which is exchange split in magnetic materials. The resonance enhancement is a re-sult of the vanishing real part of the energy denominator in second order perturbation theory. Furthermore the polar-isation of the scattered photons yields information about the intermediate states involved in the scattering process. Performing full polarisation analysis, Sanyal et al.  and Perry et al.  have shown that the dominant contribu-tion to XRES at the Er and Tb LIII edges stems from transitions 2p → 5d. Hence XRES probes mainly the po-larisation of the conduction band electrons at the LIIIedge of the rare earth metals. These electrons are supposed to mediate the interlayer coupling.
Experiments were performed at the 6ID-B beamline of the APS. The high ﬂux and the high Q-resolution al-lows a detailed study of the temperature dependence of the propagation vector τ∗ and reﬂection width. While the neutron data is resolution limited and the reﬂections over-lap strongly, the diﬀerent features can be better resolved by XRES.
Figure 9 compares the diﬀraction pattern at the LIII edge of Er and Tb, respectively, for the [Er20|Tb5] sam-ple. Because of the strong charge scattering background
0 20 40 60 80 100 120 140 T [K] 0,23 0,24 0,25 0,26 0,27 0,28 0,29 τ * [Å -1 ] X-ray Neutrons
Fig. 10. Single peak analysis of the the reﬂections in Figure 9b as a function of temperature: Modulation wave vectorτ∗ de-termined at the Tb LIIIabsorption edgeE = 7.518 keV. The neutron results are also shown.
we performed the experiment in σ → π geometry only, i.e. the polarisation of the incoming light is perpendicular to the scattering plane (σ polarisation), while the scattered light is polarised parallel to the scattering plane (π po-larisation). In contrast to charge scattering, which con-serves the polarisation, the magnetic scattering can rotate it [28, 29]. Using the (006) reﬂection of a pyrolytic graphite crystal suppressed the charge scattering at the Er LIIIedge by 95%, as the analyser 2θ angle is 85 degree. The Al (222) reﬂection yielded a charge scattering suppression of more than 99% at the Tb LIII edge (2θ ≈ 90 degree), which is mainly due to the high degree of horizontal linear polari-sation of the incoming X-ray beam. Therefore we have to measure around the (0004) Bragg reﬂection at the Er LIII edge, where the charge scattering is reduced due to the atomic form factor.
For the [Er20|Tb5] sample we observe the same type of reﬂections at both absorption edges (Er LIIIand Tb LIII). The temperature dependence of the modulation wave vec-tor is shown in Figure 10 along with the neutron data for the [Er20|Tb5] sample. The X-ray data is taken from mea-surements at the Tb LIII edge. The propagation vectors derived from the neutron and X-ray data show the same variation with temperature (Fig. 10).
The width of the magnetic reﬂections is determined completely by the coherence length of the spin polarisation for the X-ray data, the instrumental resolution can be ne-glected. We deduce a coherence length ζ = ∆Q2πz ≈ 350 ˚A or 5 bilayers. The same behaviour is observed for anti-ferromagnetic coupling of FM layers. With the onset of the FM order the intensity of the reﬂection due to mod-ulated magnetic order decreases (Fig. 11). For both types of reﬂections we observe complementary hysteresis loops as a function of temperature. The resonance behaviour shown in Figure 12 conﬁrms the magnetic origin for the modulation type reﬂections and the half integer superlat-tice satellites. The double peak structure, clearly resolved at the Er LIII edge, has not been observed in the earlier study of bulk Er , possibly due to a insuﬃcient energy resolution. 0 20 40 60 80 100 120 140 T [K] 0 0.1 0.2
Int. int. [arb. un.]
2.5-Fig. 11. Single peak analysis of the the reﬂections in Figure 9b as a function of temperature: Integrated intensities of the τ∗ and the 2.5− reﬂection measured atE = 7.518 keV.
Fluorescence 8.35 8.36 8.37 8.38 E [keV] 0 0.2 0.4 0.6 0.8 1 1.2 1.4
Int. int. [arb. units]
(0004+τ*) (0004)3.5 + Er LIII a) Fluorescence 7.48 7.49 7.5 7.51 7.52 7.53 7.54 7.55 E [keV] 0 0.02 0.04 0.06 0.08 0.1 0.12 0.14
Int. int. [arb. units]
Fig. 12. Energy dependence of the integrated intensity: (a) close to the Er LIII edge,T = 30 K, (b) close to the Tb LIII edge,T = 12 K. The ﬂuorescence yield in the upper part gives a measure for the respective edge position.
At the Tb LIIIedge, Perry et al.  observed a similar resonance behaviour, when they studied the helix phase of metallic Tb at 226 K.
In contrast, the [Er22|Tb22] sample has a qualitative diﬀerent diﬀraction pattern at the two absorption edges, shown in Figures 13a and 13b. At the Er LIII edge we
3.6 3.8 4 4.2 4.4 Q z [r.l.u] 10-5 10-4 10-3 10-2 10-1 100
Norm. Int. [arb. un.]
6 K 120 K Y +τ* 1+ 2+ 3+ 4+5+ 6+ 1 -2 -3 -4 -5 -6 -7 -8 -9 -a) [Er22|Tb22] Er LIII 7+8 + 3.6 3.8 4 4.2 4.4 Qz [r.l.u.] 10-3 10-2 10-1 100
Norm. int. [arb. un.]
6 K 240 K 0.5 -b) [Er22|Tb22] Tb LIII 1.5 -2.5
-Fig. 13. XRES as a function of Qz measured in σ → π ge-ometry at diﬀerent temperatures, normalised to the maximum intensity: (a) XRES from the [Er22|Tb22] sample close to the Er LIII absorption edge (E = 8.361 keV); (b) XRES from the [Er22|Tb22] sample close to the Tb LIII absorption edge (E = 7.518 keV).
observe a broad diﬀuse intensity τ∗at low temperature, re-lated to the short range magnetic modulation (cf. Fig. 14). The width of the feature, as deduced by a Gaussian ﬁt, equals the reciprocal Er layer thickness. On top of the broad feature, a series of sharp reﬂections appears at low temperature (see Fig. 14). They can be identiﬁed as in-teger and half inin-teger superlattice satellites. On heating, the broad feature and the sharp reﬂection disappear both roughly at 80 K. This is consistent with the loss of mag-netic order for bulk Er at this temperature: also in the multilayer we do not observe magnetic short or long range order in Er above this temperature. The resonance be-haviour at the Er LIII edge shown in Figure 15 is diﬀer-ent for the half integer and integer superlattice satellites: while the half integer satellites resonate as expected for a magnetic origin, the integer satellites show the increased absorption of a charge reﬂection. The resonance shape of the magnetic reﬂections is the same as for the [Er20|Tb5] superlattice. When magnetic ordering occurs inside the Er layer, we assume that the ferromagnetic Tb layer in-duces ferromagnetic order at the interface, while the cen-tre adopts the bulk Er-like modulated magnetic structure. The modulated structure is only short range, while the
in-4.25 4.30 4.35 4.40 4.45 0 10 20 30 Q_z [r.l.u.] Norm. int. 4.25 4.30 4.35 4.40 4.45
Fig. 14. Single peak analysis of the part of the diﬀraction pattern inside the box in Figure 13a.
8.34 8.36 8.38 Energy [KeV] 0 0.5 1 1.5
Int. int. [arb. units]
(0004+τ*) 0 0.02 0.04 0.06 0.08
Int. int. [arb. units]
(0004)7 + 0 0.02 0.04 0.06 0.08 0.1 0.12
Int. int. [arb. units]
(0004)7.5 + Er LIII a) b) c)
Fig. 15. Energy dependence of integrated intensities close to the Er LIII edge from [Er22|Tb22] superlattice, T = 9 K: (a) (0004)7.5+, (b)(0004)7+, (c) (0004 +τ∗), the broad component of the ﬁt shown in Figure 14. The absorption edge is deter-mined by a ﬂuorescence yield measurement.
terfacial order follows the long range coupling of the Tb layers.
At the Tb LIII edge, the 2l2+1 reﬂections due to anti-ferromagnetic coupled FM layers appear below 230 K (see Fig. 15b). The reﬂections can be detected for the whole temperature range of the FM phase despite the strong charge scattering background close to the (0004) central
0 20 40 60 80 100 120 T [K] 800 1000 1200 1400 1600 ξxy [Å] 500 600 700 ξz [Å] Heating Cooling 0.26 0.27 0.28 0.29 0.3 0.31 τ * [Å -1 ] 0.1 0.2 0.3 0.4 0.5
Int. int. [arb. units]
42 44 46 48 50 Φ [deg.] Phase transition Neutrons
Fig. 16. Temperature dependence (T = 10 K) of the magnetic modulation peak (0002−τ∗) in the Er0.8Tb0.2ﬁlm, determined atE = 8.359 keV, i.e. the Er LIII edge. Integrated intensities have been determined performing rocking scans across the re-ﬂection. The vertical correlation lengthζz is deduced from the width of longitudinal scans [000qz], the in-plane correlation length is deduced from the width of the rocking scans, which correspond roughly to transverse scans in reciprocal space.
reﬂection. The width of the reﬂection is about the same as the width of the structural reﬂections. The range of mag-netic order along the growth direction is therefore compa-rable to the range of structural order.
An [Er20|Tb10] sample, that has been studied only by XRES, behaves in a similar way. Short range modulated correlations are found at the Er edge, while long range FM spin polarisation is observed for energies close to the Tb edge. We detect hints to ferromagnetic coupling as well as to antiferromagnetic coupling. However, to draw conclusions on the magnetic structure for this sample, the neutron diﬀraction data is required.
The XRES from the Er0.8Tb0.2 alloy ﬁlm is very in-tense (up to 50 000 counts per second) and not obscured by the superlattice reﬂections. We studied the tempera-ture and energy dependence of the magnetic modulation at the peak (0002− τ∗) (Figs. 16 and 17). The onset of XRES intensity coincides with the N´eel temperature found by neutron diﬀraction. However, the integrated in-tensity shows two kinks as a function of temperature, one at 60 K and a second at 22 K. These are correlated with a signiﬁcant increase of the peak width, that corresponds
7.48 7.49 7.5 7.51 7.52 7.53 7.54 7.55 E [keV] 0 0.005 0.01 0.015
Int. Int. [arb. units]
10 K Tb LIII 8.31 8.32 8.33 8.34 8.35 8.36 8.37 8.38 E [keV] 0 0.02 0.04 0.06 0.08 0.1
Int. Int. [arb. units]
Fig. 17. Energy dependence (T = 10 K) of the magnetic mod-ulation peak (0002− τ∗) in the Er0.8Tb0.2 ﬁlm. Integrated in-tensities have been determined performing rocking scans across the reﬂection.
to a decrease of the correlation length. Both, the corre-lation length along the growth direction and in-plane are lowered in this temperature range. The modulation vector shows a small tendency of a hysteresis. For single crystals of the same composition Millhouse et al.  observed a stronger hysteresis and also slightly diﬀerent phase transi-tion temperatures, that can be explained by the epitaxial strains in the ﬁlm. The resonances at the Er and at the Tb edge have the same shape as in the case of the superlattice samples.
Neutron diﬀraction from a series of superlattices show basal plane ferromagnetic ordering for all investigated samples, assumed to occur mainly in the Tb layers. The phase transition temperatures for this structure depend on the thickness of the Tb layer. If the Tb layer thick-ness is greater than 20 mono-atomic layers, the ordering sets in at TN of bulk Tb. The suppression of the helix phase in Tb and Dy containing superlattices has been explained in terms of compressive strains due to the epi-taxy on the smaller ions for other rare earth superlat-tices [3, 6, 30]. With XRES, we observe weak Fourier com-ponents according to the ferromagnetic order in Er below
the ordering temperature of bulk Er, too (cp. Figs. 12, 15). We attribute this to an induced order at the interface to the Tb layers, while the exchange energy, that deﬁnes the phase transition temperature, is not changed signiﬁcantly from the bulk Er value. For Tb thicknesses smaller than 10 mono-atomic layers ferromagnetic order of the basal plane is observed only for temperatures below 60 K with a strong thermal hysteresis. Long range ordered, modulated magnetic structures exist only in the [Er20|Tb5] sample below 150 K. For the other samples we observe modu-lated phases without any coupling between neighbouring layers roughly below 80 K.
Long range order of the c-axis component occurs in the [Er20|Tb5] superlattice. To our knowledge this is observed for the ﬁrst time in a Rare Earth superlattice. The phase transition temperatures are similar to the c-axis ordering in bulk Er. In the other samples we observe a short range modulated c-axis component. The transition to a ferro-magnetic alignment of the c-component is suppressed in that cases.
The neutron diﬀraction data indicates a coexistence of a modulated magnetic phase with antiferromagneti-cally coupled ferromagnetic layers in the [Er20|Tb5] sam-ple. According to the XRES data, the modulated and the ferromagnetic structures are present in both, the Er and the Tb layers, since corresponding superlattice reﬂections were observed at the LIII resonances of both elements. Combining neutron diﬀraction and XRES results indicates that 4f and 5d electronic states show as well modulated as ferromagnetic order. Since these two ordering phenomena are mutually exclusive, they can be realized only as an incoherent superposition, i.e. a laterally inhomogeneous state. From transversal Qxscans, which were found to be resolution limited, we can conclude, that the correspond-ing domains are rather large (>800 ˚A). Such a model of a laterally inhomogeneous magnetic state could also ex-plain the large hysteresis eﬀects at low temperature. One could argue, that domain growth processes are limited by structural imperfections at the interfaces which act as pin-ning centres. To clarify this issue, we recently studied the diﬀuse scattering of polarized neutrons at grazing inci-dence .
Our structural characterisation shows, that the inter-faces are not atomically ﬂat, but exhibit strongly verti-cally correlated roughness. Therefore the nearest neigh-bour arrangement is highly anisotropic: along the growth direction a sequence of atoms corresponding to the nom-inal layer composition is closely followed. In the lateral directions a nearly random alloy is realized in the two interface regions of each layer, see the schematic in Fig-ure 18. Thus, the interfacial region can be viewed as a ‘structurally highly anisotropic alloy’. In the [Er20|Tb5] superlattice, this anisotropic alloy extends through the whole Tb layer. The strong structural anisotropy in the interface region leads to a signiﬁcantly diﬀerent phase di-agrams for the layered system and the alloy with the same nominal composition (20% Tb, 80% Er). To derive quan-titative conclusions about the magnetization distribution, e.g. the decay of a given magnetic structure in one of the
Fig. 18. Schematic view of a single layer with the two interface regions, cut along the growth direction and one lateral direc-tion. Correlated structural roughness is combined with some degree of interdiﬀusion.
layers, it would be necessary to observe a larger number of main Bragg reﬂections.
If the Tb layer thickness becomes bigger, we observe diﬀerent spin polarisations for each element. The diﬀuse XRES at the Er LIII edge points to a short range mag-netic modulation restricted to a single Er layer. At the Tb LIIIedge we were able to observe the spin polarisation according to an antiferromagnetic coupling of ferromag-netically ordered layers because of the strong suppression of the charge scattering by the polarisation analysis. The gain of magneto elastic energy due to compressive strains becomes more important for thicker Tb layers and leads to the ferromagnetic phases. The ferromagnetic Tb layers can couple via magnetic dipolar interactions , leading to the antiferromagnetic coupling, even if the Er thickness is as big as 20 mono-atomic layers.
7 Summary and conclusion
We have investigated the structural and magnetic prop-erties of [Er|Tb] multilayers. The interface roughness is vertically correlated as can be seen from the longitudinal oscillations in the diﬀuse X-ray scattering under grazing incidence.
From the reﬂectivity we get an upper limit for the in-terface extension of 3–4 mono-atomic layers. Since this is partly caused by correlated roughness, the sequence of atoms along the growth direction may still corre-spond to the nominal composition, even if the layer thick-ness becomes as small as 5 atomic layers. This conclu-sion is supported by the diﬀerent magnetic behaviour of the Er0.8Tb0.2 alloy and the [Er20|Tb5] superlattice, in which the nominal Tb layer can be considered as a highly anisotropic alloy.
The system shows diﬀerent magnetic structures de-pending on the composition of the superlattice. Antifer-romagnetic coupling of ferAntifer-romagnetic layers is present in all samples, while long range incommensurate magnetic modulations appear only in the [Er20|Tb5] superlattice. The eﬀect of the artiﬁcial superstructure is emphasised by the comparison between the Er0.8Tb0.2 alloy and the [Er20|Tb5] superlattice. While the former shows modiﬁed phase transition temperatures as compared to the bulk alloy and a common conduction band polarisation, new magnetic structures appear in the superlattice, e.g. the basal plane ferromagnetism in Er due to the anisotropic alloying at the interface. In this superlattice, we observe long range ordering of the c-axis component of the mag-netic moment. To our best knowledge this was observed for the ﬁrst time in Rare Earth superlattices. The coupling of ferromagnetic layers could be mediated via dipolar in-teractions leading to an antiferromagnetic coupling of fer-romagnetic Tb layers, which is observed in the samples containing thicker Tb layers.
In conclusion, the eﬀect of competing anisotropies is to break up long range order due to exchange interactions for larger thicknesses. A coherent magnetic order is estab-lished for the basal plane and the c-axis component if the nominal Tb layer is suﬃciently thin (5 monolayers) and the diﬀerent interface regions join.
We thank J. Thelen for the technical support during the sample preparation and E. Zoellner and D.S. Robinson for technical support and fruitful discussions during the beamtime at the APS. Use of the Advanced Photon Source was supported by the US Department of Energy, Basic Energy Sciences, Oﬃce of Science, under Contract No. W-31-109-Eng-38. The MUCAT sector at the APS is supported by the Department of En-ergy, Oﬃce of Science through the Ames Laboratory contract No. W-7405-Eng-82.
1. M.B. Salamon, S. Sinha, J.J. Rhyne, J.E. Cunningham, R.W. Erwin, J. Borchers, C.P. Flynn, Phys. Rev. Lett. 56, 259 (1986)
2. C.F. Majkrzak, J.W. Cable, J. Kwo, M. Hong, D.B. McWhan, Y. Yafet, J.V. Waszczak, C. Vettier, Phys. Rev. Lett. 56, 2700 (1986)
3. R.A. Cowley, J.M.M.M. 177–181, 1156 (1998)
4. K. Dumesnil, C. Dufour, Ph. Mangin, G. Marchal, M. Hennion, Phys. Rev. B 54, 6407 (1996)
5. J.A. Simpson, D.F. McMorrow, R.A. Cowley, R.C.C. Ward, M.R. Wells, Z. Phys. B 101, 35 (1996)
6. C. Bryn-Jacobsen, R.A. Cowley, D.F. McMorrow, J.P. Goﬀ, R.C.C. Ward, M.R. Wells, Phys. Rev. B 55, 14360 (1997)
7. J. Voigt, E. Kentzinger, U. R¨ucker, W. Schweika, W. Schmidt, D. Hupfeld, D. Wermeille, Th. Br¨uckel, Europhys. Lett. 65, 4, 560 (2004)
8. D. Gibbs, J. Bohr, J.E. Axe, D.D. Moncton, K.L. D‘Amico, Phys. Rev. B 34, 8182 (1986)
9. C.F. Majkrzak, J. Kwo, M. Hong, Y. Yafet, D. Gibbs, C.L. Chien, J. Bohr, Adv. Phys. 40, 99 (1991)
10. W. Babik, Grenzfl¨achenmorphologie von GMR und TMR-Schichtsystemen, Ph.D. thesis, RWTH Aachen (2002)
11. J. Kwo, G.K. Wertheim, M. Gurvitch, D.N.E. Buchanan, IEEE Trans. Mag. Mag. 19, 795 (1983)
12. L.G. Parrat, Phys. Rev. 95, 359 (1954)
13. D.A. Jehan, D.F. McMorrow, R.A. Cowley, M.R. Wells, R.C.C. Ward, K.N Clausen, Phys. Rev. B 48, 5594 (1993) 14. H. Zabel, Appl. Phys. A 58, 159 (1994)
15. S. Sinha, E.B. Sirota, S. Garoﬀ, H.B. Stanley, Phys. Rev. B, 38, 2297 (1988)
16. S. Nerger, E. Kentzinger, U. R¨ucker, J. Voigt, F. Ott, H. Seeck O., Th. Br¨uckel, Physica B 297, 185 (2001) 17. I.K. Schuller, Phys. Rev. Lett. 44, 1597 (1980)
18. E.E. Fullerton, I.K. Schuller, H. Vanderstraeten, Y. Bruynserade, Phys. Rev. B 45, 9292 (1992)
19. W. Sevenhans, M. Gijs, Y. Bruynserade, H. Homma, K.I. Schuller, Phys. Rev. B 34, 5955 (1986)
20. G.M. McIntyre, R.F.D. Stansﬁeld, Acta. Cryst. A 44, 257 (1988)
21. P.J. Brown, International Tables of Crystallography C (1983)
22. J.W. Cable, E.O. Wollan, W.C. Koehler, M.K. Wilkenson, Phys. Rev. 140, 1896 (1965)
23. J. Jensen, A.R. Mackintosh, Rare earth magnetism (Oxford University Press, Oxford, 1991)
24. A.H. Millhouse, W.C. Koehler, Intern. J. Magnetism 2, 389 (1971)
25. J.P. Hannon, G.T. Trammel, M. Blume, D. Gibbs, Phys. Rev. Lett. 61, 1245 (1988)
26. M.K. Sanyal, D. Gibbs, J. Bohr, M. Wulﬀ, Phys. Rev. B, 49, 1049 (1994)
27. S.C. Perry, M.M.R. Costa, W.G. Stirling, J.R. Longﬁeld, D. Mannix, Th. Br¨uckel, J. Phys.: Condens. Matter 10, 1951 (1998)
28. M. Blume, D. Gibbs, Phys. Rev. B 37, 1779 (1988) 29. J.P. Hill, D.F. McMorrow, Acta Cryst. A 52, 236 (1996) 30. R.S. Beach, J.A. Borcher, A. Matheny, M.B. Salamon, B.
Everitt, K. Pettit, J.J. Rhyne, C.P. Flynn, Phys. Rev. Lett. 70, 3502 (1993)
31. J. Voigt, E. Kentzinger, U. R¨ucker, A. Paul, T. Br¨uckel, to be published